Research Inventy: International Journal Of Engineering And ScienceVol.2, Issue 8 (March 2013), Pp 18-22Issn(e): 2278-4721, Issn(p):2319-6483, Www.Researchinventy.Com18Characterization of Polymeric Membranes under LargeDeformations by a Neural ModelFarid Hicham1,2, El Ghorba Mohamed1, Erchiqui Fouad2, M’hamed Chergui11Laboratoire de Contrôle et Caractérisation Mécanique des Matériaux et des StructuresENSEM, B.P 8118, Oasis-Route El JadidaCasablanca, Maroc2Laboratoire de Bioplasturgie et Nanotechnologie, UQAT, 445, boul. de l’Université,Rouyn-Noranda (QC), Canada J9X 5E4Abstract: Recent progress in polymers modeling shows a need for a precise description of the materialbehavior under the combined effect of the applied efforts and temperature.The Artificial Neural Networks(ANN), whose operation is based on some properties of biological neurons, contain various architecturesstrongly interrelated treating elements and offering an alternative to conventional computational approaches.They respond in parallel to a set of inputs, and are affected by transformations more than by algorithms andprocedures. They can achieve complicated operations of Input-Output without explicit relationships (linear andnonlinear) between all the presented data during a learning process.In our work, we are interested by thecharacterization of circular thermoplastic membranes, ABS (Acrylonitrile butadiene styrene), under biaxialdeformation using the free blowing technique. Hyperelastic Mooney-Rivlin model is considered. A neuralalgorithm (based on artificial neural networks) is used to model the behavior of blowing these membranes, theresults are compared with experimental studies and numerical finite differences model.Key words : membrane, Artificial Neural Networks, free blowing, hyperelasticity, ABS.I. INTRODUCTIONWorking a polymeric sheet attached by its contour in a 3D shape is the main feature of the process ofblow molding. Generally, the deformation is very fast, non-uniform, multiaxial, and occurs at a formingtemperature above the glass transition temperature . The modeling of this phenomenon remains delicate andcreates several difficulties as in the experimentation level  as in the modeling level in terms of importantcomputational time, as well as the implementation of nonlinear constitutive laws...Often, as the bubble size increases and the internal pressure approach a maximum value beyond it thereno solution, the numerical scheme diverges. So, to remedy this problem, we consider in this work, an approachbased on an artificial neural networks model , to model the behavior of thermoplastic membranes.Recently, neural networks are used in many areas include the classification, pattern recognition, speechsynthesis, diagnosis, identification and control of dynamic systems, or even to improve the quality of producedparts in various industrial processes such as injection molding or blow molding. The use of neural networks inthe identification processes is justified by the fact that they can be well approximated nonlinear functionsthrough their capacity to reproduce rather complex behavior, and their performances are improving socontinuously while relying on a dynamic learning , which provides a robust neuronal identification vis-à-visthe parametric variations and disturbances that can affect the operation of the system studied. Modeling usingneural networks requires among a model selection which is a crucial step in designing a neural network, as withany non-linear model. Indeed, this phase should lead to choose the model that has a complexity that is bothsufficient to fit the data and not excessive.In this work, the power of neural networks is used to model thenonlinear behavior in free bowing of a polymeric membrane in ABS. A multilayer neural network is used forthis application, in order to reproduce the behavior of this membrane; the results are compared withexperimentation as well as with finite difference model .II. ARTIFICIAL NEURAL NETWORKS2.1 IntroductionNeural networks have been studied since the 40s with the notion of formal neuron of McCulloch andPitts  who first developed a mathematical model of biological neuron.Hence a neural network is amathematical model of treatment consists of several basic interconnected neurons via weights that play the role
Characterization Of Polymeric Membranes Under Large…19of synapses. These weights assume values that define the behavior of the whole structure. The adaptation of thelatter through a suitable learning algorithm, allows the network to learn, memorize and generalize information.2.2 Multilayer network2.2 ArchitectureIn general, a multilayer network is composed of an input layer, an output layer, and a number of hiddenlayers. Each neuron is connected to all neurons of the next layer via connections whose weights are real.Usually, the neuron used in the hidden layers or in the output layer, performs a weighted summation of its inputsand a nonlinear transformation which is often the sigmoid function. While the neuron used in the input layer,simply passes its input to output.The architecture of a multilayer network can be given by the following figure, Fig 1 :Figure 1. Architecture of a multilayer perceptron2.3 Learning processThe learning of a neural network means that it changes its behavior to allow it to move towards aclearly defined purpose. In other words, learning is adjusting the connection weights so that the outputs of thenetwork are as close as possible to the desired outputs for all the used examples.Initially, the learning ofmultilayer networks was determined by the gradient method. Then, all optimization methods have been appliedto this problem as the conjugate gradient method, the Levenberg-Marquardt [7,8]or Kalman filters… Thus,the literature on learning of multilayer neural networks is very rich. However, we limit the study of the back-propagation algorithm combined with a Levenberg-Marquardt optimization algorithm, which is a modifiedversion of the gradient method and remains the most used and most responded. This is an optimizationalgorithm that seeks to minimize a cost function which covers the gap between the desired output and thatdelivered by the network, to expand more knowledge, we bring the reader to references  and .The back-propagation algorithm can be described using the following two phases:Propagation phase orrelaxation: initially, the input values are provided to the network’s input layer, then the network propagates theinformation from one layer to another to the output layer, and which gives the response of network.Back-propagation phase: that is to calculate the difference between the outputs of the network and the desiredresulting changes in weight of the output neurons. Then, retro-propagating the error to the input layer whichallows the adaptation of the weights of the hidden layer.In our network, we used a learning algorithm by back-propagation associated with a Levenberg-Marquardtoptimization algorithm , with a transfer function of sigmoid type.In our architecture, the error in the presentation of an example, denoted by E, can be given by the followingexpression:(1)wherein, represents the component of the desired output vector. The overall error to minimize is thesum of all errors on the database. The inputs and outputs of the neurons j and k explicit from the followingexpressions:(2)
Characterization Of Polymeric Membranes Under Large…20(3)Where f is the sigmoid activation function defined by:(4)The adjustment of the weights of the network by the back-propagation algorithm is ensured through thefollowing iterative equation:(5)With ε and i denote the pitch and the iteration number.The derivative of E with the weight depends on its position, in fact:If the weight connects the hidden layer to the output layer, so:(6)If the weight connects the input layer to the hidden layer, then:(7)It should be emphasized that the convergence of the back-propagation algorithm depends on a variety ofparameters, namely:The complexity of the database and the order of presentation of examples. Indeed, various studies haveshown that a random sample presentation allows faster learning,The structure of the neural network consideredand especially the number of neurons in the hidden layer which must not be very important to ensure thegeneralization ability of the network, or very small for the network to learn,The initial setting of the algorithmparameters, essentially the initial values of weight and iteration pitch must be chosen in a manner allowing tohave a fast convergence.The multilayer neural network that we propose has the following structure:Figure 2. Structure of the used multilayer neural networkThe used network consists of an input layer, hidden layers, and an output layer. The number of neuronsin the output layer depends on the response contemplated by the network. For the identification program, twoneurons are required in the output layer to give the response of the excitation, while the input of the network isthe variance of the corresponding pressures. As for modeling behavior of the membrane, the neuron will outputvariance in response to pressure, while the input will be presented by the stretch ratios.The experimental data areused for network learning, also, the back-propagation algorithm is used for error of perceptron learning. Thus,the optimization algorithm of Levenberg-Marquardt is used also in view of minimizing the error during theoperation of back propagation, this optimization technique is more powerful than other optimization algorithms,but it requires more memory.InputlayercontaininganexcitationvectorMultilayerneuralnetworksOutputlayercontainingaresponsevector
Characterization Of Polymeric Membranes Under Large…21III. EXPERIMENTALThe materials considered in this work is the ABS (Acrylonitrile butadiene styrene). The initial sheetthickness was 0.46mm. The exposed circular domain of radius R=3.175 cm is heated to the softening pointinside a heating chamber using infrared heaters. When the temperature was quite uniform over the flat sheet, theinflation was started using compressed air at a controlled flow rate. In most inflation tests the experiment endedwhen the bubble burst. The bubble pressure, its height at the pole and time are recorded simultaneously using avideo camera and a data acquisition system.IV. RESULTSFig 3 below shows a comparison between our neural model, finite difference model using a hyperelastic Ogdenmodel [10, 11], and experimental measurements.Figure 3. Internal pressure versus the bubble height, comparison between experimental results, finite differencemodel, and neural networks modelNote that the neural model we propose reproduces faithfully the behavior of the ABS membrane aswell as the finite difference model. The margin of error between the neural model and the experimental curveremains negligible, and can also be minimized while depending on the choice of the number of hidden layers inthe network and the chosen optimization algorithm. By increasing the number of hidden layers in the network,while keeping the same transfer function and the same optimization algorithm of Levenberg-Marquardt, theneuronal model can be adjusted for more fitting with the experimental results,Fig 4 below shows the results of model fitting:Figure 4. Internal pressure versus the bubble height, comparison between experimental results, finite differencemodel, and neural networks model (Adjusted model)It is clear that the neural model that we propose reproduces the behavior of the membrane, but, thefitting procedure that contains a number of algorithms, affects the computation time which becomes increasinglyimportant also with increasing the number of hidden layers in the network, which induces the addition of otherconditions nonlinearity.
Characterization Of Polymeric Membranes Under Large…22V. CONCLUSIONThe objective of this work is to characterize the hyperelastic behavior of thermoplastic sheets used inthe process of thermoforming, blow molding or injection blow molding, with other modeling methods thanconventional methods, by exploiting the robustness of neuronal models.The results have accentuated thestrength of the model chosen to reproduce the behavior of membranes, regardless of material or geometricnonlinearities presented in the study of such materials.A conclusion section must be included and shouldindicate clearly the advantages, limitations, and possible applications of the paper. Although a conclusion mayreview the main points of the paper, do not replicate the abstract as the conclusion. A conclusion mightelaborate on the importance of the work or suggest applications and extensions.REFERENCES Rasmussen, H. K., J. H. Christensen and S. Gottsche, Inflation of polymer melts into elliptic and circular cylinders, J. Non-Newtonian Fluid Mech. 93(2–3), 245–263, 2000 Joye, D. D., Poehlein, G.W. and Denson, C. D. A Bubble Inflation Technique for the Measurement of Viscoelastic Properties inEqual Biaxial Extension Flow, II Trans. Soc. Rheol., 16: 421–445, 1972 J. Hopfield, Neural networks and physical systems with emergent collective computational abilities. Proceeding of the NationalAcademy of sciences of the United States of America, 1982 P. Borne, M. Benrejeb, J. Haggège, Les réseaux de neurones : présentation et applications, Paris : Technip 2007 F, Erchiquiet. A, Derdouri, Analyse Expérimentale et Numérique du Analyse Expérimentale et Numérique du Comportement deMembranes Thermoplastiques en ABS et en HIPS dans le Procédé de Thermoformage, the canadian journal of chemicalengineering, vol 83, 2005 W. McCulloch, W. Pitts, A Logical Calculus of the Ideas Immanent in Nervous Activity, Bulletin of Mathematical Biophysics, vol.5, pp. 115-133, 1943 Levenberg, K. A Method for the Solution of Certain Nonlinear Problems in Least Squares, Quarterly of Applied Mathematics, 2(2):164–168, 1944 Marquardt, D. An Algorithm for Least Squares Estimation of Nonlinear Parameters, SIAM Journal on Applied Mathematics, 11(2):431–441, 1963 P. Davis, Levenberg-Marquardt Methods and Nonlinear Estimation, SIAM News, Vol. 26, Number 6, 1993 Ogden, R. W. Large Deformation Isotropic Elasticity – on the Correlation of Theory and Experiment for Incompressible RubberlikeSolids, Proc. R. Soc. Lond., A326: 565–584, 1972 F. Erchiqui, Analyse Expérimentale et Numérique du Comportement de Membranes Thermoplastiques en ABS et en HIPS dans leProcédé de Thermoformage, the canadian journal of chemical engineering, Volume 83, 2005